of 36

• date post

06-Feb-2018
• Category

Documents

• view

216

1

Embed Size (px)

Transcript of Fractal Geometry Applied To Fracture - Lehigh University Geometry Applied To Fracture ... Fracture...

• Fractal Geometry Applied To FractureJ. J. Mecholsky, Jr.Materials Science & Engineering DepartmentUniversity of FloridaGainesville, FL 32611-6400

jmech@mse.ufl.eduGlass Tutorial Series: prepared for and produced by theInternational Material Institute for New Functionality in GlassAn NSF sponsored program material herein not for sale Available at www.lehigh.edu/imi

• Log v

Log K = Log (Y c )

U

rKc

Bond Breaking Leads to Characteristic Features

• OutlineExperimental Observations - One View of Fracture

Fundamental Questions About Fracture -How does a crack propagate at all length scales?

Experimental Tools - Fractography (FSA) , Fracture Mechanics (FM) & Fractal Analysis (FA) Fractoemission (FE), Crack Velocity Measurements

Analytical Tools - Quantum Mechanics (QM),Molecular Dynamics (MD), ab initio, Monte Carlo, FEM, FD

Conclusions - FSA, FM, FA, MD & QM combine to form model of the scaled fracture process.

• Mirror

Mist

Hackle

Fracture origin

Characteristic Markings Are Observed

on the Fracture Surface

• J.J. Mecholsky, Jr., Fractography of Optical Fibers, in ASM Engineered Materials Handbook, 4, Ceramics and Glasses, Section 9: FailureAnalysis, (1992).

Relationship Holds For Large Size & Stress Range

r1/2 = constant

• Energy & Geometry Are Related

In The Fracture Process

2 = a0 [ED*]

KC = Y (c)1/2 = (2 E )1/2

= fracture energy

E = Elastic Modulus

= Fracture Stress (Strength)

C = Critical Crack Size

KC = Fracture Toughness

• Characteristic Features Aid Failure Analysis

KC = Y (c)1/2 KBj = Y (rj)1/2c = (a b )1/2 rj / c = constant

• Fracture Mechanics & Fractography Provide A Framework for Quantitative Analysis

KIC = Y c 1/2 Crack Boundary

KB1 = Y1 r11/2 Mirror-Mist Boundary

KB2 = Y2 r21/2 Mist-Hackle Boundary

KB3 = Y3 r31/2 Crack Branching Boundary

[c/rj = constant]

• FSA Can Be Applied To Single Crystals

• Slate Fracture Surface On Window Sill at Kimbull Union Academy

Courtesy of Prof. Yet-Ming Chiang

• Fracture Markings Can Last 4000 Years

Titis Sarcophagus - Egypt c. 2500 BC [Prof. Greenhut]

• Epoxy Fracture With Glass Fiber As Origin

• Glass Fiber Fractures Within Epoxy Matrix

• AISI 4340

Fracture In Steel Shows Characteristic Features

=790MPa

• Brittle Fracture Is Observed At Many Length Scales

• Brittle Fracture Can Be Observed At Many Length Scales

Courtesy of Dr. Darryl Butt [UF]

• Mirror

Mist

Hackle

Fracture origin

Characteristic Markings Are Observed

on the Fracture Surface

• Mist and Hackle Appear Similar in Shape

• Many Observations Lead To The Conclusion Of Fractal Fracture

Scaling Behavior

Self-Similarity In A Plane

Scale Invariance

• Fractal Geometry A Renewed Math Characteristics:

Non-differentiable Defined by a Fractional

Dimension (i.e. 1.3, 2.4, etc.) Self-similar features Scale invariant features

http://math.rice.edu/~lanius/frac/

• SCALING CAN BE DESCRIBED BY FRACTAL GEOMETRY Fractal Geometry is - a non-Euclidean geometry that exhibits - self-similarity (or self-affinity) & - scale invariance and is characterized by the

- fractal dimension, D.

• Replicas Provide Multiple Slit Islands for Analysis

• Log (Ruler Length)

Slope = -D*Log Length (A-B)

B

A

FRACTAL DIMENSION IS MEASURED ALONG CONTOUR

A-B = Slit Island Contour

• Material Class D* (dimensionless) Single Crystals Glasses Glass Ceramics Polycrystalline Ceramics Polymers Metals

0.07-0.12 0.07-0.1 0.06-0.3 0.06-0.35 0.2-0.29 0.06-2.5

Fractal Dimension Varies For Different Materials

J. J. Mecholsky, Jr., Fractography, Fracture Mechanics and Fractal Geometry: An Integration, Ceram. Trans. 64, in Fractography of Glasses and Ceramics III, eds. J. P. Varner, V.D. Frechette, & G. D. Quinn, Am. Ceram. Soc. (1996).

• (D*) 1/2

K ICPolycrystallineMaterials

Glass-Ceramics

Single Crystals

0.2 0.3 0.4 0.5 0.60

1

2

3

4

5

(MPa-m 1/2 )

Toughness Increases With Fractal Dimension

Kc = E a01/2 D*1/2

• D* Is Related To Flaw-to-Mirror Size Ratio

KIC = E (a01/2) D*1/2 = Y a (c)1/2 KB1= E (b01/2) = Y1a (r1)1/2 [if a0 = b0 and Y = Y1]

then, D* = c/r1

• D* Is Related To Flaw-to-Mirror Size Ratio

Mecholsky & Freiman J ACerS 74[12]3136 (1991)

• D* Is Related to Mirror-to-Flaw Size Ratio

Mecholsky & Freiman J ACerS 74[12]3136 (1991)

05

1015

0 5 10 151/D*

r1/cGlass

PyroceramZnS

SiPZTAl2O3

(Solid Line is 1:1)

• 3BaO5SiO2

D*=0.13

Kc=1.0 I

AR= 1.4

D*=0.16

Kc=1.3 I

AR= 3.6

D*=0.26

Kc=2.2 I

AR = 8

I =MPam1/2

Fracture Surfaces Polished Surfaces

Glass:

Kc = 0.7 I

D* = 0.1

• Energy & Geometry Are Related

In The Fracture Process

2 = a0 [ED*]

KC = (Ea01/2) D*1/2 = (2 E )1/2

= fracture energy

E = Elastic Modulus

D* = Fractal Dimensional Increment

a0 = Characteristic Structural Parameter

KC = Fracture Toughness

• 020406080

100

0 50 100 150

ED* (GPa)

2 (J/m2)

Glass CeramicsGlasses

Single Crystals

Fracture Behavior Appears Related To Material Class

a0 = 2/ (ED*)

• Fractal Geometry Has Been Used In Failure Analysis

Silicon [J. Mater Res 6,1248 91 ] Ocala Chert [J Mater Sci Ltrs 7, 1145 88] Intermetallics [J. Mater. Sci.6,1856 91] Si3N4 [J. Mater. Sci. 32 6317 97] Dental Glass Cer. [JACerS 78 3045 95] Epoxy Resin [Scanning 20 99 98]

2 = a0 [ED*] ; Kc = a01/2 ED* 1/2 ; D* = c/r1

• Energy & Geometry Are Related

In The Fracture Process

2 = a0 [ED*]

KC = (Ea01/2) D*1/2 = (2 E )1/2

= fracture energy

E = Elastic Modulus

D* = Fractal Dimensional Increment

a0 = Characteristic Structural Parameter

KC = Fracture Toughness

• Modeling Has to Explain Several Observations

Scaling topography (mirror, mist, etc.) self similarity (self affinity)

Fracto-emission Velocity (Chaotic) Behavior

• Much evidence exists for chaotic and fractal scaling behavior

Fracto-emission : light, particles, molecules, etc. [e.g., cf. Langford, et. al., J.Mat. Res. 4, 1272 (1989)] Dynamic instability : chaotic crack velocities at branching [e.g., cf. Fineberg, et. al., Phys.Rev.Ltrs 67,4(1991)] Self-similar fracture surfaces : crack branching [e.g., Ravi-Chandar & Knauss, Inter.J.Fracture 26,65-80(1984) Kulawansa et al., J. Mater. Res.9,2476 (1994) Mecholsky et al., Adv. In Cer.22 ACerS (1988); J. Materials Res.13 ,11 (1998).] Scaling : Energy (c) & Geometry (a0, D*) [e.g., cf. Passoja, Adv. In Cer. 22, 101 (1988) ACerS; Mecholsky, Cer.Trans. 64 385-93, ACerS (1996); West et al., J. Non-crystalline Solids, 260 (1999) 99-108; Y. Fahmy, J. C. Russ and C. C. Koch, J. Mater. Sci. 6, 1856-1861 (1991).]

• Fracture In Materials

Is there a mathematical formulation which permits insight into the fracture process at all scales?

There are several fundamental questions that need to be answered:

How do bonds break? Once a bond breaks, how do the ensembles of broken bonds propagate?